|Year : 2020 | Volume
| Issue : 4 | Page : 371-375
Inflammatory and immunogenic response of the tissue after application of freeze-dried hydroxyapatite gypsum puger scaffold compared to freeze-dried hydroxyapatite bovine scaffold
Amiyatun Naini1, Mohamad Rubianto2, Fourier Dzar Eljabbar Latief3, Achmad Gunadi1, Dewi Kristiana1, Nike Hendrijantini4, I Ketut Sudiana5
1 Department of Prosthodontic, Faculty of Dentistry, Jember University, Jember, Indonesia
2 Department of Periodontic, Faculty of Dentistry, Airlangga University, Surabaya, Indonesia
3 Physics of Earth and Complex Systems, Micro-CT Laboratory, Faculty of Mathematics and Natural Sciences Institut Teknologi Bandung, Bandung, Indonesia
4 Department of Prostodontic, Faculty of Dentistry, Airlangga University, Surabaya, Indonesia
5 Department of Electron Microscope, Faculty of Medicine, Airlangga University, Surabaya, Indonesia
|Date of Submission||09-Dec-2019|
|Date of Decision||16-Apr-2020|
|Date of Acceptance||22-Jun-2020|
|Date of Web Publication||20-Dec-2020|
Dr. Amiyatun Naini
Department of Prosthodontic, Faculty of Dentistry, Jember University, Jl. Kalimantan 37 Jember
Source of Support: None, Conflict of Interest: None
| Abstract|| |
Background: Inflammation is a mechanism or reaction of the natural immune system to defend from external hazards. All foreign objects that enter the body will trigger an immune response in the form of antibodies. In Indonesia, the prevalence of diseases that involve the inflammatory process in the body is high. Freeze-dried hydroxyapatite gypsum puger (HAGP) scaffold is a gypsum powder which is currently under development as a bone replacement material. Freeze-dried hydroxyapatite bovine (HAB) scaffold is a bone substitute material available on the market. Objective: To analyze the inflammatory and immunogenic responses in the tissue after application of freeze-dried HAGP scaffold compared to freeze-dried HAB scaffold through mediators of tumor necrosis factor alpha (TNF-α) and immunoglobulin G (IgG) in rats. Materials and Methods: This study used Wistar rats. HAGP group and HAB group were applied subcutaneously, settled for 7 and 14 days, then the levels of TNF-α and IgG were measured using enzyme-linked immunosorbent assay. Statistical analysis was done using nonparametric test with the Kruskal–Wallis test. Results: TNF-α levels at day 7 in the HAGP group were nearly equal to the control group, while those in the HAB group were higher. Statistically, the significance was P = 0.184 (P > 0.05). At the 14th day, the level of IgG on the HAGP and HAB groups the level was higher than the control group, statistically it was found P = 0.127. Conclusion: freeze-dried HAGP scaffold compared to freeze-dried HAB scaffold did not cause inflammatory and immunogenic response on rats through mediators of TNF-α and IgG.
Keywords: Freeze-dried hydroxyapatite gypsum puger scaffold, freeze-dried hydroxyapatite bovine scaffold, immunogenic, inflammation
|How to cite this article:|
Naini A, Rubianto M, Latief FD, Gunadi A, Kristiana D, Hendrijantini N, Sudiana I K. Inflammatory and immunogenic response of the tissue after application of freeze-dried hydroxyapatite gypsum puger scaffold compared to freeze-dried hydroxyapatite bovine scaffold. Contemp Clin Dent 2020;11:371-5
|How to cite this URL:|
Naini A, Rubianto M, Latief FD, Gunadi A, Kristiana D, Hendrijantini N, Sudiana I K. Inflammatory and immunogenic response of the tissue after application of freeze-dried hydroxyapatite gypsum puger scaffold compared to freeze-dried hydroxyapatite bovine scaffold. Contemp Clin Dent [serial online] 2020 [cited 2022 May 19];11:371-5. Available from: https://www.contempclindent.org/text.asp?2020/11/4/371/304144
| Introduction|| |
Inflammation is a mechanism or reaction of the body's natural immune system to fight and protect from irritants, microorganisms, and foreign objects. This process is a biological response to danger signals that threaten the body. Inflammatory responses generally occur if there is a foreign body that activates macrophages and other cells to produce and release various cytokines including tumor necrosis factor-alpha (TNF-α). In Indonesia, the number of diseases that involve inflammatory processes is quite high.,
In general, all foreign objects that enter the body will trigger the emergence of the foreign body's immune response which is referred as immunogenic or antigen, which can trigger the production of antibodies. Antibodies which are glycoproteins that produced by B cells will form immunoglobulin (Ig), There are several types of Igs, including IgG which is the most common type in the body., An example of foreign material that is often inserted into human body is bone replacement material.
Biomaterials serve as a medium to deliver inflammatory cells to the desired area and induce local tissue regeneration, acting as a barrier to protect cells implanted in tissues from host immune attacks, or as reactors to stimulate recruitment, and differentiation of the host cells. Biomaterials function as an integral component of tissue engineering that serves to provide the original extracellular matrix framework so that cell growth and tissue regeneration can take place.
Freeze-dried hydroxyapatite gypsum puger (HAGP) scaffold is a synthetic bone replacement material derived from natural gypsum powder (CaSO4.2H2O) which is being developed as a preservation material for the alveolar bone. The freeze-dried HAGP scaffold material has been successfully synthesized by characterization using scanning electron microscopy, X-ray diffraction, and degradation test on alveolar bone sockets., Freeze-dried hydroxyapatite bovine scaffold (HAB) is a bone substitute available readily on the market that is used as a comparison in this research. ,,
HAGP scaffold material as well as HAB scaffold contains hydroxyapatite. Hydroxyapatite (Ca10(PO4)6(OH)2) is a calcium phosphate crystal that provides rigidity in bone tissue.,,
In general, a safety measurement of bone replacement material that will be used as tissue preservation needs to be conducted to make sure they are biocompatible. Biocompatibility of materials can be measured in vivo by observing the inflammatory and immunogenic responses to tissue.,
The freeze-dried HAGP scaffold material has never been tested for its tissue response. Hence, it is important to conduct a research to analyze the inflammatory and immunogenic responses to tissue after application of freeze-dried HAGP scaffold in rat. The purpose of this study was to analyze the inflammatory and immunogenic responses to tissue after administration of freeze-dried HAGP scaffold through a decrease in TNF-α and IgG mediators in rat.
| Materials and Methods|| |
The research ethics test was conducted at the Faculty of Dentistry, Airlangga University. The type of research used is purely experimental. The research design used was the posttest-only control group design. This study used three groups of male Rattus norvegicus rats, aged 12–14 weeks, weighing 200–250 g (n = 5), and adapted for a week.
Preparation of freeze-dried HAGP scaffold was initialized with weighing 4 g of HAGP, diluted solid gelatin with hot water with a temperature of 600°C. The HAGP was mixed with gelatin liquid up to 10 ml, freeze-dried via freeze-drying system, crushed, milled, and sifted with particle sizes of 150–355 μm, and sterilized by Gamma radiation in BATAN. Poly ethylene glycol (PEG) then added to the HAGP scaffold, to obtain a concentration of 10% PEG we mixed liquid PEG 400 and solid PEG 4000. The resulting material then stored in a sterile container and ready for application to the subcutaneous area of rats [Figure 1].,
The rats were anesthetized intramuscularly using ketamine 100 mg/ml and xylazine base 20 mg/ml ratio 1: 1 at a dose of 0.08–0.2 ml/kg BW. After anesthetized, they were shaved clean in the back, and an incision was made in the subcutaneous area with the length of 0.5 mm then closed with stitches using DR SELLA Silk Braided usp 3/0 75 cm (in control group). Next, an incision was made in the subcutaneous area of the rat's back and augmentation was performed by inserting 0.1 ml of HAGP + PEG scaffold material and stitched. The comparison treatment group with HAB + PEG 0.1 ml augmentation was then sewn and waited for 7 and 14 days.
The rats were euthanized using 5 ml ether placed in a cotton inside a closed glass container and then the rats were inserted one by one for 5 min. An open thorax surgery was conducted to draw 2 ml of blood from the heart. Furthermore the determination of TNF-α levels on day 7 and IgG on day 14 were performed using enzyme-linked immunosorbent assay.
The data were tested for their normality using Shapiro–Wilk, and data distribution turned out to be abnormal, and the calculation continued using nonparametric test with the Kruskal–Wallis test.
| Results|| |
The TNF-α level on day 7 in the HAGP scaffold group was almost identical with the control group while in the HAB scaffold group the levels were higher. The normality test proved that the data is not normally distributed, then we used Kruskal–Wallis test (as nonparametric test) and statistically obtained P = 0.184. This means that there is no significant difference between the HAGP and HAB groups compared to the control [Table 1] and Figure 2].
|Figure 2: Bar diagram of tumor necrosis factor-alpha expression in the control group, hydroxyapatite gypsum puger scaffold and hydroxyapatite bovine scaffold|
Click here to view
The levels of IgG on day 14 in the HAGP and HAB groups both were higher than in the control group, statistically P = 0.127. This shows no significant difference between the HAGP and HAB groups compared to the control group [Table 2] and [Figure 3].
|Figure 3: Immunoglobulin G levels in the control group, hydroxyapatite gypsum puger scaffold, and hydroxyapatite bovine scaffold|
Click here to view
| Discussion|| |
Inflammatory and immunogenic responses in tissue after subcutaneous application of HAGP scaffold and HAB scaffold in rat was done by observing TNF-α expression on day 7. Results TNF-α expression in the HAGP scafold group was the same as in the control group, while in the HAB scaffold group, the expression is higher. It is clear that higher levels of TNF-α indicate an ongoing inflammatory process. TNF-α is a pro-inflammatory mediator produced by macrophages that functions to stimulate inflammatory cells, fibroblasts, and epithelial cells. Inflammatory cells have a function to eliminate nonvital tissue and prevent invasive bacterial infections.
An incision was made before administration of scaffold material in the subcutaneous region so that inflammation occurs in all groups of samples. Inflammation is the initial stage of a protective response from pathogens or foreign bodies, or injuries suffered by the host tissue. This process is characterized by vascular dilation, increased capillary permeability, increased blood flow and leukocytes. The inflammatory response is very important because it not only warns cells to engage in an immune response during infection but also initiates wound repair and healing process. Inflammation is marked by the presence of leukocytes, especially neutrophils, macrophages, and eosinophil.
A few minutes after the beginning of inflammation, the macrophages present in the tissue are histiocytes within the subcutaneous tissue. Macrophages will exclude important factors in inflammation such as TNF, interleukin-1, factors that stimulate granulocyte-monocyte colonies, monocyte colony-stimulating factors (CSFs) and CSF granulocytes. These factors are formed by macrophages that are activated in the tissue that undergoes inflammation, and a small number of others are formed by a network of inflamed cells, resulting in the increase of TNF-α.
Statistical analysis between the HAGP, HAB, and control groups resulting in P = 0.184. This shows that the HAGP and HAB groups compared to the control group were not significantly different. This means none of them induce an inflammatory response compared to control because the HAGP scaffold and the HAB scaffold contain the basic ingredients of hydroxyapatite. Hydroxyapatite material is a bioactive ceramic that has good biocompatibility and bioactivity properties, it is an excellent material used for new bone growth and able to accelerate the regeneration process of damaged bones. Hydroxyapatite in scaffold has a strong ability to stimulate cell proliferation and induce osteogenic differentiation. Scaffolds consisting of hydroxyapatite biomaterials have excellent ability in the formation of fibrous tissue between the bone implants.
TNF-α levels on day 7 are associated with osteoclast precursor recruitment and differentiation into adult osteoclasts in the defect. This is supported by other researchers that the defects are associated with TNF-α expression from the surface of osteoclast markers.
Determination of immunogenic response to tissue after application of HAGP scaffold and HAB scaffold in rat subcutaneous layer was done by observing IgG expression on day 14. Observations made on day 14 because immune reactions that cause rejection of graft material transplantation are usually happened within 10–14 days. In this study, the expression of IgG in the HAB scaffold group was higher than the HAGP scaffold and control group. This was because the HAB scaffold was hydroxyapatite from bovine bones containing protein. Exposure to this kind of protein can increase the response of IgG. The higher the amount of protein exposure, the higher the amount of IgG antibodies produced. According to Bratawidjaja and Iris (2014) the first (primary) antigen exposure activates T cells and B cells, B cells then differentiate and proliferate to produce small amounts of IgG. Whereas repeated exposure (secondary) with the same antigen will increase the proliferation of B cells to produce more IgG. IgG antibodies are the front line of adaptive immunity and specific humoral response in the body against pathogens.,
Statistical analysis between the HAGP, HAB, and control scaffold groups results in P = 0.127. This shows that there was no significant difference between the HAGP and HAB groups compared to the control, which means that they did not cause an immunogenic response compared to the controls. This is because the HAGP and the HAB scaffold contain the main ingredients of hydroxyapatite. Hydroxyapatite material is biocompatible, low toxicity, biodegradable, nonimmunogenic, and noncarcinogenic. bioceramic based composite material and has a potency as a biodegradable bone implant.
| Conclusion|| |
Freeze-dried HAGP scaffold does not cause an inflammatory and immunogenic response to rats through mediators of TNF-α and IgG compared to freeze dried HAB scaffold.
The authors would like to thank to research grant supporting the IDB program University of Jember in 2019.
Financial support and sponsorship
Conflicts of interest
There are no conflicts of interest.
| References|| |
Janeway Charles A, Travers P, Walport M, Shlomchikn M. Immunobiology. Sec. 2-4. New York: Garland Science; 2001.
Baratawidjaja KG, Rengganis I. Immunologi Dasar. Edisi ke-11. Fakultas Kedokteran Universitas Indonesia; 2014. p. 52
Abbas L. Basic Immunology. Functions and Disorders of the Immune System. 2nd
ed. Canada: WB Saunders Co.; 2006. p. 34.
Kearney CJ, Mooney DJ. Macroscale delivery systems for molecular and cellular payloads. Nat Mater 2013;12:1004-17.
Lee EJ, Kasper FK, Mikos AG. Biomaterials for tissue engineering. Ann Biomed Eng 2014;42:323-37.
Tal H, Zvi A, Roni K, Ilan B, Goshen G. Augmentation and Preservation of the Alveolar Process and Alveolar ridge of Bone. Department of Periodontology and Dental Implantology. Tel Aviv University Israel; 2012. p. 25-30.
Naini A, Ardhiyanto HB, Yustisia Y. Proses sintesis dan karakterisasi hydoxyapatite menggunakan analisis XRD FTIR dari gypsum puger kabupaten jember sebagai material augmentasi ridge alveolar. J Stomatognatic (J. K. G Unej) 2014;11:32-7.
Naini A, Sudiana IK, Rubianto M, Ferdiansyah, Mufti N, Characterization and degradation of hydroxyapatite gypsum puger (HAGP) freeze-dried scaffold as a graft material for preservation of the alveolar bone socket. J Internat Dent Med Res 2018;11:532-6.
Mahyudin F, Djoko R, Fedik AR. Aulaniam. Regenerasi pada massive bone defect dengan bovine hydroxyapatite sebagai scaffold mesenchymal stem cell. JPB 2011;13:179-95.
Manalu JL, Soegijono B, Indrani DJ. Characterization of hydroxyapatite derived from bovine bone. Asian J Appl Sci 2015;3:758.
Puspa KA, Asmi D. Sintesis dan karakterisasi biokeramik hidroksiapatit bahan tulang sapi pada suhu 800-1100. J Teori dan Aplikasi Fisika 2014;2:125.
Surbakti A, Oley MC, Prasetyo E. Perbandingan antara penggunaan karbonat apatit dan hidroksiapatit pada proses penutupan defek kalvaria dengan menggunakan plasa kaya trombosit. J Biomed 2017;9:137-40.
Darwis D, Warastuti Y. Sintesis dan karakterisasi komposit hidroksiapatit (Ha) sebagai graft tulang sintetik. J Ilmiah Aplikasi Isotop dan Radiasi 2008;4:143-4.
Mozartha M. Hidroksiapatit dan aplikasinya di bidang kedokteran gigi. Cakradonya Dent J 2015;7:807-68.
Mahyudin F, Hermawan H. Biomaterial and Medical Devices: A Perspective from an Emerging Country. Switzerland: Springer; 2016. p. 54-5.
Poedjijarti T. Biokompatibilitas Scaffold Hidroksiapatit-Kitosan-Kondroitin Sulfat Secara in vivo
Sebagai Bone Graft. Thesis Thesis, Sekolah Pasca Sarjana. Universitas Airlangga; 2018.
Desai LS, Lister L. Biocompatibility Safety Assessment of Medical Devices: FDA/ISO and Japanese Guidelines Toxikon Corp. (Bedford, MA, USA): Toxikon Corp; 2003. p. 7-8.
KresnoadiU. Toll-Like Receptor 2 Sebagai Signaling Pathway Osteogenesis Tulang Alveolar Yang di Induksi Kombinasi Aloe Vera dan Graft. Disertasi. Fakultas Kedokteran Universitas Airlangga; 2012.
Kumar V, Abbas AK, Aster JC, Robbin SL. Robbins Basic Pathology. 9th
ed. Philadelphia: Saunders; 2013. p. 17-21.
Marcelo OF, Thomas EV. Natural resolution of inflammation. Periodontol 2013;63:149-64.
Katrin D, Mayer B, Yan B. Clash of the cytokine titans: Counter-regulation of interleukin-1 and type I interferon-mediated inflammatory responses. Cell Mol Life Sci 2017;14:22-35.
Liu M, Kalbasi A, Beatty GL. Functio laesa: Cancer inflammation and therapeutic resistance. J Oncol Pract 2017;13:173-80.
Hall J. Guyton dan Hall Buku Ajar Fisiologi Kedokteran Editors: M Widjajakusumah Antonia Tanzil Paperback. 12th
ed. Singapore: Elsevier (Singapore) Pte Ltd Page Count.; 2014. p. 1172.
Herliansyah MK, Candra M, Alva ET. Natural bioceramics bone graft: A comparative study of calcite hydroxyapatite, gypsum hydroxyapatite, bovine hydroxyapatite and cuttlefish shell hydroxyapatite. Proceed Asia Pacific Indust Eng Manag Syst Confer 2012;2:1137-46.
Li Y, Zhang Z, Zhang Z. Porous chitosan/nano-hydroxyapatite composite scaffolds incorporating simvastatin-loaded PLGA microspheres for bone repair. Cells Tissues Organs 2018;205:20-31.
Khoiriyah M, Cahyaningrum SE. Sintesis dan karakterisasi bone graft dari komposit hidroksiapatit/kolagen/kitosan (HA/Coll/Chi) dengan metode ex-situ
sebagai kandidat implan tulang. Unesa J Chem 2018;7:25-9.
Cardemil C, Elgali I, Xia W, Emanuelsson L, Norlindh, Qmar Q, et al
. Strontium-doped calcium phosphate and hydroxyapatite granule promote different inflammatory and bone remodelling responses in normal and ovariectomised rats. Plos One 2013;8:1-17.
Male D, Brostoff J, Roth DB, Roit I. Immunologia. Polish ZJ, editor. Elsevier Urban & Partner: Wroclaw; 2006. p. 59-86.
Irawan B. Chitosan dan aplikasi klinisnya sebagai biomaterial. Indonesian J Dent 2005;12:146-51.
Ulum MF, Arafat A, Noviana D, Yusop AH, Nasution AK, Abdul Kadir MR, et al
. In vitro
and in vivo
degradation evaluation of novel iron-bioceramic composites for bone implant applications. Mater Sci Eng C Mater Biol Appl 2014;36:336-44.
[Figure 1], [Figure 2], [Figure 3]
[Table 1], [Table 2]